Journal of Encapsulation and Adsorption Sciences, 2017, 7, 40-66 http://www.scirp.org/journal/jeas
ISSN Online: 2161-4873 ISSN Print: 2161-4865
DOI: 10.4236/jeas.2017.71003 March 6, 2017
Adsorption-Desorption of BTX (Benzene, Toluene and O-Xylene) on Fe, Fe-Al Pillared Clay
Laboratory of Materials and Catalysis, Department of Chemistry, Faculty of Exact Sciences, University of Djillali Liabes, Sidi Bel Abbes, Algeria
Abstract The studies are conducted in laboratory to determine the adsorption-desorp- tion behavior of BTX (benzene, toluene and o-xylene) in gas phase on Fe, Fe-Al pillared clays adsorbents. In experimental conditions of constant at- mospheric pressure, initial concentrations with an increasing volume (0.5 - 2 ml) injected benzene (2.25), toluene (1.89) and o-xylene (1.66) μmol/L at T (40˚C, 60˚C and 80˚C), and the adsorption increases with increase of temper- ature, indicating that the adsorption process would be a chemical adsorption rather than physical one. The results are shown that the BTX adsorption data fitted very well (R2 > 0.999) to the both equations Langmuire and Elovitch for the three samples: bentonite (B), Fe-bentonite ( Fe B ) and Fe-Al/bentonite ( Fe Al B− ). At 80˚C, the BTX adsorption capacity increased in the following order: B Fe B Fe Al B< < − . The maximum adsorption capacity ( mq ) at 80˚C is 175.13, 171.84 and 171.81 μg/g respectively for benzene, toluene and o-xylene for Fe Al B− ; the last is a good adsorbent of BTX removal. The benzene diffuses faster than toluene and o-xylene. Thermodynamic parame- ters, such as G∆ , H∆ and S∆ are also discussed and the results sug- gested that the BTX adsorption on all samples used is a spontaneous and en- dothermic process. Desorption studies show that BTX is very easily desorbed with Fe Al B− .
Keywords Fe, Al-Pillared, Benzene, Toluene, O-Xylene, Adsorption
The natural gas and oil industry activities are known for some time to create harmful air emissions that emit volatile organic compounds (VOCs) and oxides of nitrogen (NOX), which are precursors to tropospheric ozone. The major
How to cite this paper: Mèçabih, Z. (2017) Adsorption-Desorption of BTX (Benzene, Toluene and O-Xylene) on Fe, Fe-Al Pil- lared Clay. Journal of Encapsulation and Adsorption Sciences, 7, 40-66. https://doi.org/10.4236/jeas.2017.71003 Received: January 5, 2017 Accepted: March 3, 2017 Published: March 6, 2017 Copyright © 2017 by author and Scientific Research Publishing Inc. This work is licensed under the Creative Commons Attribution International License (CC BY 4.0). http://creativecommons.org/licenses/by/4.0/
http://www.scirp.org/journal/jeas https://doi.org/10.4236/jeas.2017.71003 http://www.scirp.org https://doi.org/10.4236/jeas.2017.71003 http://creativecommons.org/licenses/by/4.0/
VOCs, the benzene, toluene and xylene (BTX) volatile compounds are signifi- cant environmental concern and are listed as priority pollutants by the United States Environmental Protection Agency (US EPA)  because of their toxic and carcinogenic effects on humans. Besides, the benzene is already known as the leukemia agent in humans . Another, VOCs characterized by their photo- chemical activity could undergo a series of photochemical reaction to from the secondary organic aerosol, which is one of the major components of airborne fine particles. The VOCs cause environmental concerns about their toxicity and malodor, even at very low concentrations, due to the obvious impacts on at- mosphere and human health; it is necessary to limit and control this air emis- sion. The difficulty, for decreasing the VOCs in gas phase at very low concentra- tions, requires a highly optimized process. Various processes can be used for ab- atement of VOCs which are broadly classified into two types: destruction (bio- filtration, thermal oxidation, catalytic oxidation, reverse flow reactor) and re- covery (adsorption, condensation, membrane separation) . The adsorption by solid adsorbents is one of the best solutions for this treatment; the choice of ad- sorbent depends on these adsorptive properties and availability. Granular or powdered actived carbon is the most widely used adsorbent , but their use is usually limited due to their high cost. Over several decades, many researchers show their interests in searching for low-cost adsorbents with excellent adsorp- tion characteristics, such as zeolites , organokaolinite , smectite , hecto- rite , organosilica , and montmorillonite  . The pillared interlayer clay (PILC) attracts attention of many researchers, and constitutes one of the most widely studied series among the microporous materials with a wide range of potential applications in adsorption processes. PILCs are formed by insertion of polynuclear inorganic cation into their interlayer space, followed by calcina- tions to give stable metal oxide pillars (e.g. Al2O3, Fe2O3 etc.) having larger mi- cropores. The purpose of this paper is to present the effectiveness of (Fe, Fe-Al)-pillared bentonite clay adsorbents to reduce the concentration of BTX and determine behavior of BTX with evaluating the influence of the temperature on BTX adsorption. Adsorption isotherm is measured at three different temper- atures: 40˚C, 60˚C and 80˚C.
2. Materials and Methods 2.1. Materials
The natural clay used in this work is a bentonite type from Maghnia (west Alge- rian). It is supplied by the Algeria Bentonite Company (ENOF). The natural bentonite is purified in laboratory  , using a sedimentation method to obtain the < 2 μm montmorillonite rich faction. The carbonates are removed by sodium acetate/chloridric acid, iron oxide by sodium thiosulfate/sodium chlo- ride and organic materials by hydrogen peroxide (30% vol.). To ensure complete transformation into the sodium from all samples, they are washed several times with 0.5 M NaCl. The exchange capacity or CEC 91 meq/100g (by methylene bleu exchange).
2.2. Preparation of Hydroxyl-Al
The pillaring solution of Al and Fe polycation are prepared separately . 0.207 M NaOH solution is added slowly while stirring to a 0.207 M AlCl3 solution un- til it reached an 3OH Al + molar ratio of 2.5 in the mixture. The mixture is aged at room temperature during 6 days at room temperature.
2.3. Preparation of Hydroxyl-Fe
Fe polycations solution is prepared by slowly adding a 0.1 M NaOH solution to 0.1 M FeCl3 solution under vigorous stirring, until the 3OH Fe + ratio reaches the value 2.5. The mixture is aged for two weeks at room temperature .
2.4. Preparation of Fe-Al Pillared Bentonite
The pillaring solution containing hydroxyl-Al oligocations and hydroxyl-Fe oli- gocations are slowly added under vigorous stirring into the suspension purified bentonite while, until the mass ratio of M3+ (M3+ = Fe3+, Al3+)/caly reached 6.25% . The solids are filtered and washed with deionized water until it are free of Cl− ions. The solids B, Fe B and Fe Al B− are calcined for 2 h at 300˚C ground and sieved.
High-purity BTX: benzene (99 wt.%, Aldrich), toluene (99.5 wt.%, Aldrich) and o-xylene (99 wt.%, Aldrich) are used absorbate.
The Analysis of the chemical composition of the purified bentonite is obtained fluorescence X. The surface area is measured with a Micromeritics ASAP 2010 instrument by adsorption of nitrogen at 77 K. Before measurement, the samples are degassed under vacuum of 20.8 Pa at 120˚C for 2.
2.6. BTX Adsorption Kinetics
1 g of the samples in the nacelle is placed in glass enclosure (10 L), closed and thermostated degassed for 2 h using the means of a water-jet pump. Then, 2 ml of BTX (benzene, toluene and o-xylene) containing respectively, 2.25, 1.89 and 1.66 μmol/L is sprayed into the enclosure by injection (Figure 1). After, the na- celles are removed from the enclosure and the samples are weighed. The expe- riments are carried out at 40˚C, 60˚C and 80˚C in a temperature controlled bath (Figure 1).
2.7. Equilibrium Isotherm
1 g of the samples in the nacelle is placed in glass enclosure (10 L), closed and thermostated degassed for 2 h using the means of a water-jet pump. Then, dif- ferent volume ranging from (0.5 - 2 ml) is sprayed into enclosure by injection of liquid BTX: benzene, toluene and o-xylene with initial concentration respective- ly 2.25, 1.89 and 1.66 μmo/L. The experiments are carried out at 40˚C, 60˚C and 80˚C in a temperature controlled bath (Figure 1). After reaching the adsorp- tion equilibrium, the nacelles are removed from the enclosure and the samples
Figure 1. Experimental set-up for the adsorption of the BTX.
weighed by Sartorius 1219 MP balance type (accuracy ± 10−3 g). The amount of adsorbed BTX on adsorbents (qe μg/g) is calculated as follows:
( )0 e e
C C V q
m − ⋅
where 0C and eC are the initial and equilibrium BTX concentrations (μg/L), respectively; V is initial liquid volume (L) equal to glass enclosure volume; and m is the adsorbent weight (g).
2.8. Desorption Experiments
For desorption experiments, the nacelle in glass enclosure is subjected before to degassing for 2 h at constant pressure. 1 g of the samples are saturated in ben- zene, toluene and o-xylene of concentration 2.25, 1.89 and 1.66 μmol/L respec- ti